Journal of the European Ceramic Society 21 (2001) 1981–1984 www.elsevier.com/locate/jeurceramsoc Barium perovskites as humidity sensing materials M. Viviani a,*, M.T. Buscaglia a, V. Buscaglia a, M. Leoni a, P. Nanni b a Institute for Physical Chemistry of Materials, National Research Council, via De Marini 6, 16149 Genoa, Italy b Department of Process and Chemical Engineering, University of Genoa, P.le Kennedy Pad. D, 16129 Genoa, Italy Received 4 September 2000; received in revised form 23 October 2000; accepted 15 November 2000Abstract The response to humidity of porous ceramics with composition BaMO3, with M=Ti, Zr, Hf or Sn, was studied. Samples wereobtained by cold isostatic pressing and sintering of ﬁne powders prepared by wet chemical synthesis. Sensitivity and response timehave been obtained by electrical impedance measurements realised in diﬀerent conditions of relative humidity (R.H.) at 25 C. Anincrease of both capacitance and conductivity with humidity was observed in all samples with open porosity. Sensitivity increasedwith R.H. and decreased with frequency, indicating a major contribution from the surface of crystals exposed to water vapour,particularly in BaTiO3 where 4000% change in permittivity was registered over the range 20–80% R.H. Time response was in thetypical range of capacitive humidity sensors, with fast (10–100 s) equilibration time for intermediate values of R.H. # 2001 ElsevierScience Ltd. All rights reserved.Keywords: BaTiO3 and titanates; Impedance; Perovskites; Sensors1. Introduction aﬀected by adsorption of impurities at the surface that must be removed by periodic thermal cycling.1 The measurement of humidity has received great atten- Ceramic materials used for detection of humidity aretion during the last two decades due to the recognised represented by metal oxides, for which diﬀerent mechan-importance of water partial pressure in many industrial isms of conduction in a humid environment have beenprocesses and in the market of air-conditioning systems reported, each corresponding to a class of sensors, i.e.for the automatic regulation of living environments.1 ionic, electronic, solid electrolites and heterocontacts.1,2 A number of humidity sensors is nowadays available Whatever the origin of impedance variation, thebased on the measurement of electrical impedance (resis- interaction with water can be described by means oftance or capacitance) of sensing materials exposed to the three basic phenomena, represented by the formation ofatmosphere. In general, commercial sensors are intended a chemically adsorbed layer of OHÀ ions bonded toto operate in relatively narrow ranges of humidity and/or metal ions at the oxide surface, the successive growth oftemperature, as all materials investigated for this pour- a multilayer of physisorbed H2O molecules and the fur-pose show good characteristics under certain conditions ther condensation of liquid water into pores with size inbut also limitations outside. For example, sensors based the mesopore range (1–250 nm).3on polymeric organic ﬁlms possess high sensitivity in the Contributions to surface conductance can be expectedwhole range of relative humidity (0–100% R.H.), but from both protons (H+) hopping between adjacent H2Ocannot be operated at high temperature and require adsorbed molecules (Grotthus chain reaction) and elec-temperature compensation. On the contrary, ceramic- trolysis of the condensed liquid. In addition, an electro-based sensors can be used over a wider temperature nic type conductance in the bulk is likely to arise fromrange, especially at high temperature, but are seriously electrons released from surface states after the chemical adsorption of water molecules.4 The possibility of reor- ientation under an external ﬁeld of molecules in the * Corresponding author. Tel.: +39-010-6475-703; fax: +39-010- physically adsorbed layer has to be also considered as6475-700. an explanation to the variation of capacitance with E-mail address: firstname.lastname@example.org (M. Viviani). humidity.0955-2219/01/$ - see front matter # 2001 Elsevier Science Ltd. All rights reserved.PII: S0955-2219(01)00155-8
1982 M. Viviani et al. / Journal of the European Ceramic Society 21 (2001) 1981–1984 Perovskite-type oxides, well known and used as dielec- Table 1trics, ferroelectrics, semiconductors and high-tempera- Composition and microstructural parameters of samples investigatedture ionic conductors, have been also considered for their Sample Composition Sintering temperature Grain size Drelresponse to humidity, one of the main advantages of (nominal) ( C)/time (h) (mm) (%)such compounds being the possibility to obtain sensing BT1 BaTiO3 1250/8 2 91materials that can be operated both at low temperature BT2a BaTiO3 1250/8 10 91(100 C) as ionic sensors and at higher temperatures BTL BaTiO3+0.3 at.% La 950/2 0.2 68(ﬃ 400 C) as semiconductors. A few paper report the BZa BaZrO3 1380/0.5 0.6 88modiﬁcations to electrical behaviour induced by BH BaHfO3 1500/2 0.6 91humidity in BaTiO3,5,6 Ba0.5Sr0.5TiO3,7,8 CaTiO39 and BS BaSnO3 1700/2 9 59SrSnO3,10 generally in the form of porous bulk ceramics a Refers to powders prepared by the solid-state route.and added with alkali or La atoms at concentrations of1–5 mol%. Recently the a.c. and d.c. electrical responseto humidity was investigated on BaTiO3 porous cera- were annealed in air at 600 C for 1 h in order to reducemics obtained from ﬁne powders prepared by a low- contact resistance. All characterisations were carried outtemperature chemical synthesis.11 In this work the into a cell at room temperature containing the sample,observations have been extended to diﬀerent Ba per- connected to a frequency response analyser (Solartron,ovskites obtained by the same chemical route and, for SI1260) and a commercial humidity/temperature sensorcomparison sake, to some materials prepared by con- (Rotronic, Hygroclip-S, polymeric capacitive type,ventional solid state reaction. Experimental results are response time 410 s). The relative humidity inside thepresented and discussed according to the surface proto- chamber was regulated by mixing two streams of drynic conduction model. and wet nitrogen gas. The capacitance and the con- ductance of the sample were recorded at ﬁxed frequency as a function of time for step variations of R.H., while2. Samples preparation the whole impedance spectrum (10À2–107 Hz) was mea- sured at ﬁxed R.H. and after long equilibration time Powders with composition BaMO3 (M=Ti, Hf, Sn) (30 min). Sensitivity was calculated from data as ÁC/were prepared through the reaction between Ba(OH)2 Cm, i.e. capacitance variation relative to the minimum(98%, main impurity Sr) and the chloride or oxychlor- measured in dry conditions.ide of the relevant tetravalent cation (99.9%), in aqu-eous solution and with the addition of NaOH at 80 Cunder atmospheric pressure.12,13 Chlorine was totally 3. Results and discussionremoved before drying by washing at room temperaturewith distilled water, while some amount ($800 ppm) of XRD on sintered samples in all cases revealed thesodium was detected in the powders by plasma spectro- presence of the perovskite-like phase only, with tetra-metry (ICP). gonal symmetry in BaTiO3 and cubic in other oxides at For comparison sake, samples of BaTiO3 and BaZrO3 room temperature. The average grain size, evaluatedwere prepared by solid-state reaction at high tempera- from SEM images of sintered samples after polishingture using BaCO3 and TiO2 or ZrO2. In this case the and thermal etching is reported in Table 1.concentrations of both Na and Cl impurities were below The relative variation of capacitance with humidity is100 ppm. A doped composition was also obtained, by shown in Fig. 1 for diﬀerent specimens. All samplesadding 0.3 mol% of La(NO3)3 to a chemically prepared present a good sensitivity when R.H. is above 50–60%,BaTiO3 powder (see Table 1) by wet ball milling in but huge diﬀerences appear at lower humidity levels. Inplastic jar with zirconia balls. particular, for BH the relative variation in capacitance Cylindrical greens were formed by cold isostatic is higher than 10% already at the lowest R.H. mea-pressing at 150 MPa and sintered in air at diﬀerent sured, whereas for others it is limited to a few per centtemperatures in order to obtain porous ceramics and, in up to 50% R.H. The capacitance measurements repor-the case of BaTiO3, to obtain diﬀerent pore size dis- ted in Fig. 1 substantially follow an exponential depen-tributions. Sintered bodies were analysed by X-ray dif- dence with humidity described by the formulafraction (XRD, Philips, PW1710), scanning electron microscopy (SEM, Philips 515) and N2-adsorption por- ÁCðR:H:Þ C À Cm ln ¼ ln ¼ ÀAðR:H:M À R:H:Þosimetry (Micromeritics, ASAP2010). The electrical ÁCmax CM À Cmresponse to humidity was investigated by a.c. electrical ð1Þimpedance measurements on disk-shaped samples (dia-meter=10 mm, thickness=1 mm), electroded with Ag– where CM and Cm represent the maximum and thePd–Al paste. Before measurement, electroded samples minimum capacitance respectively, R.H.M the humidity
M. Viviani et al. / Journal of the European Ceramic Society 21 (2001) 1981–1984 1983 The time response to humidity has been investigated by recording the impedance after the application of a step-like variation of R.H. The assumption of instanta- neous equilibration of the humidity is supported by the use of ﬂuxing gas as carrier of water vapour, ensuring a total replacement of the testing environment in less than 1 s. The variation of capacitance as a function of time (C(t)-C(0)) was compared with two exponential func- tions with diﬀerent time constants ( 1, 2) expressed by CðtÞ À Cð0Þ ¼ k1 ð1 À eÀt=1 Þ þ k2 ð1 À eÀt=2 Þ ð2ÞFig. 1. Capacitance sensitivity vs. relative humidity. Data were col-lected at 1 kHz for the BT series and at 20 kHz for other samples. The results of non-linear ﬁtting of experimental data with the Eq. (2) are reported in Table 2. It is importantvalue for which C=CM and A is a quantity related to to remark that the time constants are substantially thethe spreading of sensitivity. The expression (1) is not same during adsorpion and desorption and are notvalid when C=Cm and when the capacitance is not inﬂuenced by the actual values of humidity. Only ataﬀected by humidity variation but it is useful to plot toge- very high R.H. levels (90%) a slowing down of thether and compare the behaviour of materials with very response is observed. Eq. (2) can be explained by thediﬀerent sensitivities: the lower A, the wider is the humidy existence of two distinct processes with diﬀerent activa-range over which the capacitance variation is distributed, tion energies and kinetic constants (Fig. 3). Alternatively,meaning a better response of the material. Results of linear the existence of one single process of interaction amongﬁtting on data of Fig. 1 are reported in Table 2 together water molecules and solids that develops under variouswith the relative capacitance variation over the range 20– conditions (two as a ﬁrst approximation), can be80% R.H. It can be seen that samples with lower sensi- assumed. From spectroscopic experiments on defectivetivity have also a narrower spreading of sensitivity, even single crystals surfaces14 it is known that chemisorptionthough for BaHfO3 wide spreading and quite low sensi- in perovskites is likely to be completed at a water pres-tivity have been found and BTL shows the highest sure of the order of 0.1 Pa, and for this reason can be dis-capacitance variation on a relatively narrow range. carded at higher humidity levels. On the contrary, physical The frequency dependence of capacitance at various adsorption and capillary condensation take place in thehumidity levels is reported in Fig. 2 for the sample BT1. whole range and the time required to reach equilibriumA dispersion of sensitivity is clearly observed at low can be related to the time necessary for the H2O pres-frequencies (below 100 Hz in this sample). This feature sure to establish into the various parts of the solid. As ais common to all samples, to both ﬁne and coarse- consequence, microstructure and particularly size dis-grained BaTiO3 and also to paraelectric Stannate, Zir- tribution of pores must be considered to explain theconate and Hafniate, indicating that the capacitive electrical properties presented here. As can be seenresponse to humidity is mainly due to surface processes comparing data in Table 2, the ﬁrst response time islike physisorption and condensation, and is not strictly determined by the amount of mesopores, being shorterconnected to the electrical properties of crystals (e.g. in samples with little porosity in that range. From sizeferroelectricity). Further conﬁrmation comes out from distributions of pores (Table 3) it is also possible toconductance data, that present the same behaviour.Table 2Relative mesopore speciﬁc volume (Vmesopores/Vpores), sensivityspreading index (A), relative capacitance sensitivity (ÁC/Cm), and timeconstants of the response relative to a humidity step variation (ﬃ 15%)Sample Vmesopores/Vpores A ÁC/Cm 1 2 (%) (%)À1 (%) (s) (s)BT1 12.9 0.077 154 12 650BT2 11.5 0.117 11 15 250BTL 24.7 0.098 3560 220 1000BZ 7.1 0.127 65 8 45BH 32.4 0.038 84 25 190BS 12.0 0.121 5 7 170 Fig. 2. Frequency dependence of capacitance for diﬀerent R.H. in the sample BT1.
1984 M. Viviani et al. / Journal of the European Ceramic Society 21 (2001) 1981–1984 in the mesopore range, as supported by the index of spreading of sensitivity found in BaHfO3. Due to the high values of permittivity and sensitivity obtainable, BaTiO3 can be considered for the realisation of ceramic capacitive humidity sensors. Acknowledgements The authors are grateful to Professor P. Mantas of Aveiro University (Portugal) and Professor L. MitoseriuFig. 3. Time dependence of capacitance for a step variation of relative of Iasi University (Romania) for the fruitful discussionshumidity (10%) in the sample BTL. Experimental data are ﬁtted with about data interpretation and measurement methodology.Eq. (2) and single components are also reported ( 1=220 s, 2=1000 s).Table 3 ReferencesVolume (V) pore size distribution in the mesopore range (1–250 nm).Intervals of pores width (r) are expressed in nm 1. Traversa, E., Ceramic sensors for humidity detection: the state- of-the-art and future developments. Sensors and Actuators B,Sample V(r6) V(6r20) V(20r60) V(60r250) Vmesopore 1995, 23, 135–156. (%) (%) (%) (%) cm3 gÀ1 2. Nenov, T. G. and Yordanov, S. P., Ceramic Sensors. Technomic, Basel, 1996, p. 74–75.BT1 26 6 7 62 2.12E-03 3. Gregg, S. J. and Sing, K. S., Adsorption, Surface Area and Por-BT2 32 3 8 57 1.89E-03 osity. Academic Press, London, 1992, p. 113.BTL 9 46 13 32 1.92E-02 4. Fagan, J. G. and Amarakoon, V. R. W., Humidity sensors. Am.BZ 11 5 9 75 6.14E-03 Ceram. Soc. Bull., 1993, 72, 119–130.BH 9 5 7 79 3.91E-03 5. Hwang, T. J. and Choi, G. M., Humidity response characteristicsBS 0 0 0 100 1.17E-02 of Barium Titanate. J. Am. Ceram. Soc., 1993, 76, 766–768. 6. Wang, J., Xu, B., Liu, G., Liu, Y., Wu, F., Li, X. and Zhao, M., Inﬂuence of doping on humidity sensing properties of nanocrys-conclude that a uniform distribution is beneﬁcial in talline BaTiO3. J. Mater. Sci. Lett., 1998, 17, 857–859.giving a good spreading of sensitivity. These considera- 7. Holc, J., Slunecko, J. and Hrovat, M., Temperature character-tions particularly apply to BH and BTL samples which istics of electrical properties of (Ba,Sr)TiO3 thick ﬁlm humidityhave the biggest relative mesopore volume, long time sensor. Sensors and Actuators B, 1995, 26–27, 99–102.constant ( 1) and lowest A. The second time constant is 8. Yeh, Y. C. and Tseng, Y., Analysis of the d.c. and a.c. propertiesless clearly related to the microstructural properties, of K2O-doped porous Ba0.5Sr0.5TiO3 ceramic humidity sensor. J. Mater. Sci., 1989, 24, 2739–2745.even though it can be noted that the lowest t2 values are 9. Chang, A. and Tseng, T. Y., Humidity-sensitive characteristics ofrelated to reduced amount of mesoporosity (BZ) or to CaTiO3 porous ceramics. J. Mater. Sci. Lett., 1990, 9, 943–944.large average pore size (BS). Accordingly, the slowest 10. Shimizu, Y., Shimabukuro, M., Arai, H. and Seiyama, T.,response time is found in the sample with the highest Humidity-sensitive characteristics of La3+-doped and undopedamount of porosity of width below 20 nm. SrSnO3. J. Electrochem. Soc., 1989, 136, 1206–1210. 11. Caballero, A. C., Villegas, M., Fernandez, J. F., Viviani, M., Buscaglia, M. T. and Leoni, M., Eﬀect of humidity on electrical response of porous BaTiO3 ceramics. J. Mater. Sci. Lett., 1999,4. Conclusions 18, 1297–1299. 12. Leoni, M., Viviani, M., Nanni, P. and Buscaglia, V., Low-tem- perature aqueous synthesis (LTAS) of ceramic powders with The capacitive response to humidity of diﬀerent per- perovskite structure. J. Mater. Sci. Lett., 1996, 15, 1302–1304.ovskites has been investigated. Samples with general 13. Nanni, P., Viviani, M. and Buscaglia, V., Synthesis of dielectriccomposition BaMO3 (M=Ti,Zr,Hf,Sn) were prepared ceramic materials. In Low and High Dielectric Constant Materialswith very diﬀerent microstructural features, i.e. density, and their Applications, Vol. 1, ed. H. S. Nalwa. Academic Press,grain size and pore size distribution. The highest sensi- San Diego (CA), 1999, pp. 429–455.tivity and good sensitivity spreading index was found in 14. Henrich, V. E., Electron spectroscopic determination of the elec- tronic, geometric and chemisorption properties of oxide surfaces.highly porous BaTiO3 with the addition of 0.3 at.% of In Surfaces and Interfaces of Ceramic Materials, ed. L. C. Dufour,La. The major factors aﬀecting the sensitivity and C. Monty and G. Petot-Ervas. Kluwer Academic Publishers,response time were porosity and pore size distribution Dordrecht, 1989, pp. 1–28.